SyntheticMetals 103 (1999)
STM spectroscopy of (TMTSF),PF, K. Ichimura’, 0. Abe’, K. Nomura’, S. Takasakib, J. Yamadab, S. Nakatsujib, H. Anzaib
‘Division of Physics, Hokkaido University, Sapporo 060-0810, Japan bDeparment of Material
Science, Himeji Institute of Technology, Hyogo 678-1201, Japan
Abstract The SDW phaseof (TMTSF),PF, wasinvestigatedby the electrontunnelingspectroscopyusinga low temperatureSTM. At room temperature and86K, the tunnelingconductanceis almostflat indicatingmetallicstate.Below Tsow= 11.5K, the spectrumshowsthe clear gap structureassociated with the SDW state.The conductance curve is well explainedby the meanfield approximationfor the quasi-one dimensionalconductors.The SDW gapparameterdsowandco,which characterizes the transferenergyalongthe b-axis,areestimatedas A,,,=2.5-2.9 meV and~,=2.0-2.6meV, respectively.The SDW-insulator-SDW tunnelingspectrumwasalsoobserved. Keylvords: atomic force microscopy, scanning tunneling microscopy, metal-insulator phase
1. Introduction It is well knownthat a lot of quasi-onedimensional conductors undergothe densitywave (DW) condensate, which is the charge densitywave (CDW) or the spin density wave (SDW), as the groundstate[l]. In suchcondensate phaseof quasi-one dimensional conductors, manyexperiments havebeendeveloped.However,the exactshapeof the electronicdensityof statesfor the DW statehas beenunclear,sincetherewas lessspectroscopic measurement to elucidatethe electronicdensityof states. The electron tunneling is the most usetil spectroscopyin investigatingsuchcondensate stateasDW andsuperconductivity  because of itshigh energyresolution.Additionally, it is easyto analyzethetunnelingdata:the tunnelingdifferentialconductance givestheelectronicdensityof statesdirectly.Theelectrontunneling study on the quasi-onedimensionalconductorwasenergetically developedin the CDW stateof NbSe, which is oneof the most well-knowninorganicquasi-one dimensional conductors.Fomelet al.  reportedthe tunneling differential resistanceof NbSe,insulator-lead junction underpressure.They claimedthat the gap width decreases with increasingpressurewhile ratio of the gapto the transitiontemperature is constant.Ekino et al.  reportedabut the both junctions of NbSe,-insulator-Auand NbSe,-insulatorNbSe,. They explainedtheir resultsby the meanfield theory for quasi-onedimensionalconductors . In organic quasi-one dimensional conductors, the superconducting phase of (TMTSF),ClO, wasstudiedby thejunction method. Among tunnelingmethods,STM spectroscopy hasadvantages dueto itsnon-contacting tip configuration.Thereislessdisturbance to the samplesurface.The movabletip enablesto probethe local electronicstatewith atomicspatialresolution. In the presentarticle,we reportthe electrontunnelingstudyin the SDW stateof (TMTSF),PF,, which is oneof the mostfamous quasi-onedimensionalorganic conductors,by using an low
temperature STM. 2. Experimental Singlecrystalsof (TMTSF),PF,, which areribbonshapealong the a-axis, were synthesizedelectro-chemically.The SDW transitiontemperaturewasdeterminedasTs,,=l1.5 K from the resistive transition. As-grown surfaceof the a-b plane were investigatedby low temperatureSTM. 3. Resultsand Discussion Figure 1 showsthe temperaturedependence of the tunneling differential conductanceobtainedat the a-b surfaceof single crystals.As shownin thefigure,thereis somenoisein spectra.The tunnelingcurrentin the presentexperimentwasnot stabilizedwell, partiallydueto lesssurfacequality.It isdifficult to preparethe fresh surface,sincesinglecrystalsof (TMTSF),PF, areeasilybrokenby a little stress.However, we could successfullyobtain tunneling spectrabothin thenonnalandSDWstate.At roomtemperature and T=86 K, the tunneling differential conductanceis almostflat, indicatingthe metallicstate.At T=2.9K, below T,,,=ll.5 K, the spectrumshowsthe cleargapstructureassociated with the SDW state.Theconductance at zerobiasvoltageis well reducedto about 30 % of the normalconductance.The gap edgeis observednear Y=4.5mV asthe enhancement of the conductance. At first, we tried to explainthe obtainedtunnelingspectrumby the BCS density of states.Although the broadeningof the oneelectron level is taking into account,the remainedconductance insidethe gap is not explainedby the isotropicgap. The gap anisotropy is strongly suggested.However, the d-wave gap anisotropy,whichisgapless, cannotexplainthe obtainedspectrum. In order to searchfor the origin of the gap anisotropy,we examinethemeanfield theoryfor quasi-one dimensional conductors . Theelectronicbandin TMTSF saltsis almostonedimensional
0379~6779/99/$ - seefrontmatter0 1999ElsevierScience S.A. All rightsreserved. PII: SO379-6779(98)00455-X
et al. I Synthetic
0 20 Voltage (mv)
Fig. 1. Temperature dependence of the tunneling differential conductance The zero conductance line of each curve is shifted by one division for clarity.
electronic band is represented by the parameter eO,which is related with 1, and characterizes the imperfectness of the nesting. The conduction band is separated to two parts by the gap in the SDW state. In the case of imperfect nesting, the band dispersion of both split bands is undulated along k with the amplitude of co Therefore, the electronic density of states is strongly modulated. Huang et al.  proposed the calculation of the density of states in such an imperfect nesting DW state. The density of state spectrum in DW state has the finite gap of ASDW-~O,where d,, is the SDW gap parameter and enhancement at dSoW+~, instead of AsDw for the BCS prediction. We analyze the obtained tunneling spectrum according to the above calculation and the mean field theory developed by Yamaji 173.As shown Fig. 2, in the obtained spectrum peak structure appears at 4.6 mV, corresponds to A,,,+%. A sDWis scaled to the transition temperature Z’, expected for the perfect nesting. The relation between T&T, and ddSDW is given . Then we obtain parameters as A,,,,,=2.5 meV and ~,=2.0 meV. The calculated density of states using above parameters is represented by the solid line in Fig. 2. Although the fitting is not always satisfactory, the qualitative behavior is explained by the model. From the fitting to the spectrum of different sample, we obtain as A,,, =2.8 meV and f0=2.6 meV. The present estimated Asow is consistent with the one obtained by the infrared absorption as 2.5-4.3 meV . We observed another type of the tunneling spectrum, in which gap width is slightly larger and the conductance near zero bias is less than that described above. Since these spectra are often observed when we made tip contact to the sample, these spectrum is possibly due to the SDW-insulator-SDW tunneling. If small sarnpie flakes are attached to the STM tip by contacting tip to the sample surface, the SDW-insulator-SDW tunneling would be possible. In the SDW-insulator-SDW tunneling spectrum, it is expected that the peak structure and an anomaly appear at 2A,,,, and 2(A aDw+eO),respectively 151,The observed peak structure at V=S mV, corresponds to 2AsDw, is consistently explained with the above estimated A,,,v. In summary, we succeeded to obtain the tunneling differential conductance in the SDW state of (TMTSF),FP, using low temperature STM. The tunneling spectrum is qualitatively explained by the mean field theory for quasi-one dimensional conductors. By the fitting, the gap and imperfectness parameters are estimated as A,,,=2.5-2.9 meV and ~,=2.0-2.6 meV, respectively. We also obtained the SDW-insulator-SDW tunneling spectrum. Acknowledgment This work was carried out as a part of ‘Research for the Future’ project, JSPSRFTF97POO105, supported by Japan Society for the Promotion of Science.
Voltage (mV) Fig. 2. Fitting of the calculation described in the text to the tunneling conductance at 2.9 K. along a -axis. A band calculation predicted that the Fermi surface consists of a pair of slightly undulated sheet . The transfer energy along the b-axis ti, is not negligible. Therefore, the two dimensionality in band structure must be considered. Consequently, the Fermi surface is additionally modulated and the nesting of the Fermi surface becomes imperfect. The two dimensionaiity of the
References [l] G. Gruner, Density Waves in Solids, Addison-Wesley, 1994  I. Giaever, Phys. Rev. Lett., 5, (1960) 147.  A. Fournel, J. P. Sorbier, M. Konczykowski, P. Monceau, Phys. Rev. Lett., 57 (1986) 2199.  T. Ekino, J. Akimitsu, Physica B, 194-196 (1994) 1221.  X. Z. Huang, K. Maki, Phys. Rev. B, 40-(1989) 2575,  H. Bando, K. Kajimura, H. Anzai, T. Ishiguro, G. Saito, Mol Cryst. Liq. Cry%, 119 (1985) 41.  K. Yamaji, J. Phys. Sot. Jpn., 51 (1983) 1861. [S] P. M. Grant, J. Physique, 44 (1983) C3-847.  K. Kornelsen, J. E. Eldridge, G. S. Bates, Phys. Rev. B, $8, (1987) 9162.